Tables 262-263. 

 TABLE 262. — Specific Heat of Various Solids.* 



241 



Solid. 



Alloys : 



Bell metal 



Brass, red 



" yellow 



80 Cu-i-20 Sn 



88.7 Cu+i 1.3 Al •. . 



German silver ........ 



Lipowitz alloy: 24.97 Pb + 10.13 Cd + 50.66 Bi 

 + 14-24 Sn . . . . 



Rose's alloy : 27.5 Pb+48.9 Bi+23.6 Sn 



Wood's alloy : 25.85 Pb + 6.99 Cd + 52.43 Bi + 



1473 ^n 



" " (fluid) 



Miscellaneous alloys : 

 17.5 Sb+29.9 Bi+i8.7 Zn+33.9 Sn . . . 



37.1 Sb+62.9 Pb 



39.9 Pb-|-6o.i Bi 



" (fluid) 



63.7 Pb+36.3 Sn 



46.7 Pb+53.3 Sn 



63.S Bi+36.2 Sn 



46.9 Bi+53.1 Sn 



Gas coal 



Glass, normal thermometer 16™ 



" French hard thermometer .... 



" crown 



'• flint 



Ice 



India rubber (Para) 



Paraffin 



It 



u 



« fluid 



Vulcanite 



Temperature 



15-98 

 O 



o 



14-98 



20-100 



O-IOO 



5-50 



100-150 



—77-20 



20-89 



5-50 



100-150 



20-99 

 10-98 



16-99 

 144-358 



12-99 



10-99 



20-99 



20-99 

 20-1040 

 19-100 



10-50 



10-50 



-188 252 



—78 188 



—18 78 



?-ioo 

 -20- +3 

 —19- +20 



0-20 



35-40 



60-63 



Specific Heat. 



0.0858 

 .08991 

 .08831 

 .0862 

 .10432 

 .09464 



•0345 

 .0426 

 .0356 



.0552 



.0352 

 .0426 



•05657 

 .03880 

 .03165 

 .03500 

 .04073 

 .04507 

 .04001 

 .04504 



•3145 



.1988 



.1869 



.161 



.117 



.146 



.285 



•463 



.481 



•3768 



•5251 



•6939 



.622 



.712 



•3312 



Authority, t 



R 

 L 



R 

 Ln 

 T 



M 



S 



M 



R 

 P 

 R 



W 



Z 



H M 



D 



G-T 

 R W 



B 

 AM 



• These specific heat tables are compiled partly from more extended tables in Landolt-Bbrnstein-Meyerhoffer's Tables, 

 t For references see Table 263, page 242. 

 Smithsonian Tables. 



